**Understanding hopping transport and **

**thermoelectric properties of conducting **

**polymers **

### Siarhei Ihnatsenka, Xavier Crispin and Igor Zozoulenko

**Linköping University Post Print **

### N.B.: When citing this work, cite the original article.

### Original Publication:

### Siarhei Ihnatsenka, Xavier Crispin and Igor Zozoulenko, Understanding hopping transport and

### thermoelectric properties of conducting polymers, 2015, Physical Review B. Condensed Matter

### and Materials Physics, (92), 3, 035201.

### http://dx.doi.org/10.1103/PhysRevB.92.035201

### Copyright: American Physical Society

### http://www.aps.org/

### Postprint available at: Linköping University Electronic Press

**Understanding hopping transport and thermoelectric properties of conducting polymers**

S. Ihnatsenka,*_{X. Crispin,}*†*_{and I. V. Zozoulenko}*‡*

*Laboratory of Organic Electronics, ITN, Link¨oping University, SE-60174 Norrk¨oping, Sweden*
(Received 26 February 2015; revised manuscript received 19 May 2015; published 6 July 2015)
*We calculate the conductivity σ and the Seebeck coefficient S for the phonon-assisted hopping transport in*
*conducting polymers poly(3,4-ethylenedioxythiophene) or PEDOT, experimentally studied by Bubnova et al.*
[**J. Am. Chem. Soc. 134**,16456(2012)]. We use the Monte Carlo technique as well as the semianalytical approach
based on the transport energy concept. We demonstrate that both approaches show a good qualitative agreement
*for the concentration dependence of σ and S. At the same time, we find that the semianalytical approach is not in*
a position to describe the temperature dependence of the conductivity. We find that both Gaussian and exponential
*density of states (DOS) reproduce rather well the experimental data for the concentration dependence of σ and S*
giving similar fitting parameters of the theory. The obtained parameters correspond to a hopping model of localized
quasiparticles extending over 2–3 monomer units with typical jumps over a distance of 3–4 units. The energetic
disorder (broadening of the DOS) is estimated to be 0.1 eV. Using the Monte Carlo calculation we reproduce the
activation behavior of the conductivity with the calculated activation energy close to the experimentally observed
one. We find that for a low carrier concentration a number of free carriers contributing to the transport deviates
strongly from the measured oxidation level. Possible reasons for this behavior are discussed. We also study the
effect of the dimensionality on the charge transport by calculating the Seebeck coefficient and the conductivity
for the cases of three-, two-, and one-dimensional motion.

DOI:10.1103/PhysRevB.92.035201 *PACS number(s): 72.80.Le, 72.20.Ee, 72.20.Pa*

**I. INTRODUCTION**

During recent years the development of technologies using
waste heat to produce electricity, such as thermoelectric
gen-erators, has been receiving increasing attention [1]. The figure
*of merit, ZT* =*σ S _{κ}*2

*T*, describes the efficiency of the

*thermo-electric power generation; here σ is the thermo-electrical conductivity,*

*Sis the Seebeck coefficient, κ is the thermal conductivity, and*

*T* is the temperature. The conducting organic polymers have
recently emerged as promising materials for thermoelectric
applications [1–7]. These materials are cheap, of high natural
abundance, and environmentally friendly. A record high
*figure-of-merit ZT value for organic material at room temperature*
[4–6] has prompted further interest to explore this class of
materials for thermoelectric applications aiming at achieving
*the same ZT value as for the best inorganic materials.*

Among all conducting polymers, poly(3,4-ethylenedioxythiophene) (PEDOT) has become the material of choice for many applications including thermoelectric ones [8]. This is because PEDOT has a low thermal conductivity, is stable under ambient conditions, is easily processed, has a high electrical conductivity, and can even exhibit a metallic behavior at room temperature [9,10]. Despite a massive experimental attention to the electric and thermoelectric transport in PEDOT thin films, many fundamental aspects of charge mobility in this and related materials still remain poorly understood and the interpretation of many experiments remains controversial. It is generally accepted that charge carriers in PEDOT are positively charged spin-carrying polarons and spinless bipolarons resulting from interaction of excess charges with a local

*_{siarhei.ihnatsenka@liu.se}

*†*_{xavier.crispin@liu.se}
*‡*_{igor.zozoulenko@liu.se}

distortion of a PEDOT polymer backbone [4,11,12]. It was
also shown that a morphology of PEDOT films strongly
affects the character of charge dynamics, even though the
relative importance and respective role of various structural
components (conjugated backbone, counterions, chain breaks,
defects, etc.) in determining the carrier mobility remains to
be clarified [4,13–19]. Pristine polymeric films show the
increase of the conductivity as a function of temperature
following the activated [2,3] or stretched exponential
dependence [15,16,19]. This behavior is attributed to
the phonon-assisted hopping transport. Treatment of the
pristine PEDOT by solvents or polar compounds leads to
the impressive increase of conductivity by several orders
of magnitude [4,13–19]. This is also accompanied by the
change in the character of the temperature dependence of
*the conductivity exhibiting a decrease of σ as T increases,*
indicating the insulator-to-metal transition with the bandlike
character of charge transport. Note that different studies report
different temperature dependence of the high conducting
states with microscopic interpretation still being under current
debate [15–19].

An efficient control and optimization of the thermoelectric
properties of conducting polymers can be achieved using
an electrochemical transistor [3,4,20]. An active part of this
device consists of a conducting polymer channel separated
from a gate by an electrolyte with mobile anions and cations.
Without an applied gate voltage the channel is in its pristine
*highly conducting state and the source-drain current ISD*
is high. An application of the positive gate voltage forces
cations from the electrolyte to penetrate the polymer channel.
As a result, the channel is gradually reduced (i.e., the
concentration of polarons/bipolarons in polymer chains is
*decreased) resulting in a decrease of ISD*. The distinct feature
of the electrochemical transistor as compared to a conventional
organic field-effect transistor [21] is that in the former the
electronic transport occurs within the bulk whereas in the latter

it takes place along an interface. Thus, the electrochemical transistor allows us to probe the bulk thermoelectric properties of an electrochemically active material.

In the present work we focus on the theoretical
analy-sis of the thermoelectric properties of the PEDOT in the
electrochemical transistor experimentally studied recently by
*Bubnova et al. [*3]. The activated character of the temperature
dependence of the conductivity in the device at hand suggests
a thermally assisted hopping. In order to calculate the
con-ductivity and the Seebeck coefficient we perform extensive
Monte Carlo calculations complemented by a semianalytical
treatment employing a concept of the transport energy [22–24].
The Monte Carlo technique is widely used for calculations
of the conductivity in systems with the hopping transport.
Following pioneering works of B¨assler [25] on simulation
of the electronic conductivity in amorphous organic films, a
number of studies have utilized the Monte Carlo technique
for the calculations of electronic transport in a wide range of
polymeric devices including solar cells, light-emitting diodes,
and field-effect transistors [26–28]. Note that calculations
reported in the above studies correspond to diluted systems
out of the thermal equilibrium when the Fermi energy
does not enter the theory. On the contrary, thermoelectric
properties of conducting polymers are interesting at high
oxidation levels (up to 40%) for which the system is in the
thermal equilibrium and the Fermi level is well defined. In the
present work we also utilize the Monte Carlo technique in order
to calculate the conductivity and the Seebeck coefficient. It
should be mentioned that a standard expression for the Seebeck
coefficient widely used in the literature [29,30] is obtained
within the relaxation time approximation in the Boltzmann
approach, which is appropriate for the band transport. In
the present paper we derive an expression for the Seebeck
coefficient valid in a general case regardless of the particular
mechanism of transport.

It is rather difficult to perform a systematic analysis and fitting of experimental data using the the Monte Carlo method as it requires extensive computational resources. In contrast, such analysis can be easily done using the semianalytical approaches based on the transport energy concept [22–24]. In this paper we compare these two methods and demonstrate that they show a good qualitative and, for some values of parameters, even quantitative agreement. Having established this, we use the semianalytical approach to fit the experimental data of Ref. [3] to extract parameters of the system. This allows us to analyze a shape of the density of states (DOS), as well as to provide a microscopic interpretation of the hopping mechanism identifying an extend of the polaron/bipolaron quasiparticles and their average hopping distance in the structure under consideration. Finally, we investigate how the dimensionality of the motion affects the observed properties of the system and report the results of the Monte Carlo calcula-tions for the Seebeck coefficient and conductivity for the cases of two-dimensional (2D) and one-dimensional (1D) transport.

**II. MODEL**

In order to model the electrical conductivity and the Seebeck coefficient of the system at hand we adopt a standard model of the phonon-assisted hopping widely used

for the description of the charge transport in conducting
polymers [22–27]. We assume that charge carriers jump
between the localized sites of a lattice; at this point we
specify neither the precise microscopic structure of the lattice
sites nor the nature of the charge carriers. The results of
our calculation and the comparison to the experimental data
will shed light on these important issues and therefore we
postpone a related discussion to Sec.III. The phonon-assisted
*transition probability between two sites i and j with the energy*
*difference W* *= Ej* *− Ei* *separated by a distance R is given*
by the Miller-Abrahams formula [31–33],

*νij* =
*ν*0exp
−*2R*
*α* −
*W*
*kT*
*,* *W >*0
*ν*_{0}exp−*2R _{α}*

*,*

*W*0

*,*(1)

*where the localization length α describes an extend of the*
*wave function of a localized state, k is the Boltzmann constant*
*and ν*0is the intrinsic attempt-to-jump rate, which depends on
the strength of the electron-phonon coupling and the phonon
density of states.

We assume that charge carriers are in equilibrium and
*described by the Fermi-Dirac distribution function fF D(E)*
*with the Fermi energy EF.*Taking into account the occupation
probability of the initial state, and nonoccupational probability
*of the final state, the average transition rate from site i to site*

*j*reads [31,32]

*ij* *= νijfF D(Ei*)[1*− fF D(Ej)].* (2)
Throughout this work we shall neglect an electron-electron
interaction, except to allow no more than one electron to
occupy a single site.

In our calculations of the conductivity and the Seebeck coefficient we utilize two commonly used shapes of the DOS in conducting polymers, the Gaussian [22–26],

*g(E)*= √ *N*0
*2π σ*DOS
exp
− *E*2
*2σ*2
DOS
*,* (3)

and the exponential ones [34],

*g(E)*= *N*0
*2σ*DOS
exp
− *|E|*
*σ*_{DOS}
*,* (4)

*where N*0*is the concentration of sites, and σ*DOSsets a scale for
the energetic disorder (the broadening of the DOS). Note that
it is still debated in the literature which of these DOS better
reproduces the experimental results [24].

*We calculate the conductivity σ and the Seebeck coefficient*

*S* using the Monte Carlo technique and the semi-analytical
approach utilizing the so-called transport energy concept.
(A detailed description of these approaches is given in
Appendixes Band C.) The Seebeck coefficient is given by
the expression (see AppendixA),

*S(T )*= *EF− E*trans

*|e|T* *,* (5)

where the transport energy is defined as the averaged energy weighted by the conductivity distribution

*E*_{trans}=
*Eσ(E,T )*−*∂fF D*
*∂E*
*dE*
*σ(T )* *,* (6)

*and the total conductivity at a given temperature being σ (T )*=

*dEσ(T ,E)(−∂fF D*

*∂E* *).*

Note that using the Sommerfeld expansion (see, e.g., Ref. [29]), the Seebeck coefficient, Eqs. (5), (6), can be rewritten in an alternative form

*S*= −*π*
2* _{k}*2

*BT*3

*|e|*

*∂*

*∂Eln[σ (T ,E)]|E=EF.*(7) This expression (sometimes called the Mott formula) is valid

*in the limit kBT*

*E − EF, where E is the energy of states*involved in the conductivity. It follows from the Mott formula that the energy dependence of the Seebeck coefficient is primarily determined by the logarithmic derivative of the DOS at the Fermi energy. Indeed, using the Einstein relation [35,36],

*σ(T ,E)= e*2*g(E)D(E),* (8)
and substituting it into Eq. (7), we obtain,

*S*∝*d(ln g)*

*dE* *+ g*

*d(ln D)*

*dn* *.* (9)

*Because the diffusion coefficient D(E) is practically *
indepen-dent of the electron density (or only weakly depenindepen-dent on it),

*dD*

*dn* *≈ 0, the Seebeck coefficient is expected to vanish when*
the DOS has a maximum.

**III. RESULTS AND DISCUSSION**

**A. Comparison of the Monte Carlo and the semianalytical**
**approach based on the transport energy concept**

The kinetic Monte Carlo technique provides a direct mod-eling of the hopping transport in organic semiconductors and therefore it gives the most accurate description of the electronic conductivity. Its disadvantage is that it demands extensive computational resources, which makes it difficult to use this technique to analyze and fit experimental data. In contrast, such analysis can be easily done using the semianalytical approach based on the transport energy concept [22,23] (see AppendixBfor its brief description). This approach, however, utilizes various approximations concerning an averaging of the escape rates, hopping distances, etc. To be able to rely on this semianalytical approach for the analysis of the experimental data, in this section we present a comparison of the conductivity and the Seebeck coefficient based on the Monte Carlo (MC) and the semianalytical (sa) methods.

We performed extensive calculations for various values of
parameters of the system at hand and we found that the larger
*the localization length α, the better agreement between the*
Monte Carlo results and the semianalytical calculations based
on the transport energy concept. This is illustrated in Fig.1,
which shows calculations for two representative cases of large
*and small localization lengths, α= a and α = 0.2a. We first*
note that the Monte Carlo calculations based on the definition
[Eq. (5)] and on the approximate Mott formula [Eq. (7)] lead
to qualitatively similar behavior of the Seebeck coefficient, see
Figs.1(c),1(d)*. In both cases SMC*_{exhibits a monotonic growth}
with energy and, according to the expectations [see Eq. (9)],
*it vanishes when the DOS reaches a maximum at E*= 0.
However, our calculations show that quantitative difference
between these two cases can be significant, and therefore in

-0.4 -0.2 0.0 0.2 0.4 0.0 0.5 1.0 1.5 -4 -2 0 2 4 -1000 -500 0 500 1000 0 50 100 -4 -2 0 2 4 semi-analytics Monte Carlo Etr ans (eV) EF S (mV/K) (S/cm)

Fermi energy ( _{DOS}) Fermi energy ( _{DOS})

x10 -3 DOS (a) (c) (e) (b) (d) (f) Monte Carlo Eq. (7)

Monte Carlo, Eq. (5)

=a =0.2a

FIG. 1. (Color online) The Monte Carlo and semianalytical
*cal-culations of (a) the transport energy E*trans, (b) the Seebeck coefficient,

(c) the conductivity for different values of the localization length
*α= a (left), α = 0.2a (right). The DOS is given by the Gaussian,*
Eq. (3* ), which is indicated in gray in (e), (f). EF* is in units of

*σ*DOS*. σ*DOS*= 4kT , T = 300 K. In semianalytical calculations ν*0=

1012_{s}−1_{was used; for Monte Carlo calculations ν}MC

0 *= 2.3×10*13s−1

*(e), νMC*

0 *= 4.1×10*

14_{s}−1 _{(f). Here and hereafter (unless stated}

otherwise) the numerical Monte Carlo calculation are performed on the lattice 50×50×50 with a lattice constant a = 1 nm and the results are averaged over 16 different samples.

*our subsequent discussion we will present results for SMC*
based on the exact definition, Eq. (5).

*Let us now compare Ssa* _{and S}MC_{. It is seen from}
Figs.1(c),1(d) that they exhibit a qualitative agreement for
*all values of the parameter α. For large α (left panel), Ssa*_{and}

*SMC*_{show not only qualitative, but even a relatively good }
*quan-titative agreement in the energy interval E < 0 (corresponding*
*to the relative carrier concentration n/N*0* 0.5). For higher*
energies (and thus for the higher concentrations) the difference
*between Ssa* _{and S}MC_{increases. (Note, however, that such}
high concentrations are never achieved in experiments.) As
*the parameter α decreases, the functional dependencies Ssa*
*and SMCremain very close to each other, but Ssa* gets shifted
*with respect to SMC*_{[Fig.}_{1(d)}_{].}

*The difference between Ssa _{and S}MC*

_{can be traced back to}

*the difference in the corresponding transport energies, Esa*

trans
*and EMC*

trans, Figs.1(a),1(b)*. For α* *= a they are close to each*

*other in the energy interval E < 0. For smaller α the agreement*
between the transport energies worsens. Note that at low
*energies the E*trans is practically independent of the electron
energy and is situated close to the maximum of the DOS [i.e.,
*close to E*= 0 in Fig.1(a)] [24]. When the energy is increased
*such that the position of EF* approaches the DOS maximum,

*the transport energy E*trans becomes energy dependent and
*starts following the position of EF*. This behavior can be easily
understood from the fact that the transport energy plays the
role similar to that of the mobility edge [24]. The hopping
downward in energy takes place mostly from the states lying
*above E*trans, whereas the hopping upward in energy occurs
*mostly from the states situated below E*trans. As a result, as soon
*as EFis moved upward and approaches E*transfrom below, the
latter shifts upward accordingly because otherwise all states
*below E*trans would be filled and thus unavailable for energy
*jumps downwards. For higher energies, E > 0, the difference*
*between Esa*_{trans} *and E*_{trans}*MC* increases, which translates into the
*corresponding difference between Ssa _{and S}MC*

_{.}

Figures1(e),1(f) show a comparison of the Monte Carlo
*and the semianalytical conductivity σ (E) as a function of the*
Fermi energy for the case of the Gaussian DOS, Eq. (3). For
*the large localization length (α= a), σscand σMC* show not
only qualitative but rather a good quantitative agreement. As
expected from the Einstein relation, Eq. (8), the conductivity
closely follows the DOS. For low localization lengths the
*agreement between σsc _{and σ}MC*

_{worsens, see Fig.}

_{1(f)}

_{. While}

*for energies E 0, σsc*

_{and σ}MC_{remain relatively close to}each other, the deviation between them (as well as a deviation

*between the shapes of σsc*

_{and DOS) increases with increase}

*of E.*

It is important to stress that the semianalytical expression
*for the conductivity includes a fitting parameter η [see*
Eq. (B4)], which is arbitrarily chosen to adjust the magnitude
*of the σsc _{. (Note that alternatively one can set η}*

_{= 1 and adjust}

*a parameter ν*0.) This means that one can only compare the functional dependencies of the conductivities, adjusting the

*magnitude of σsc*

_{by a proper choice of η (or ν}0). In contrast,
the semianalytical expression for the Seebeck coefficient does
*not include this fitting parameter and thus a comparison of Ssa*
*and SMC _{is performed without adjusting the magnitude of S}sa*

_{.}We carried out a comparison of the Monte Carlo and semianalytical approaches for the conductivity for different

*temperatures and we found that the fitting parameter η is*

*not a constant but is temperature dependent, η= η(T ). Its*temperature dependence is not provided by the theory. This means that the semianalytical approach is not in a position to describe the temperature dependence of the conductivity. In particular, we find that for large carrier concentration

*σsc* decreases with increase of the temperature, which is in
a stark contrast to the experimental findings as well as to
the Monte Carlo calculation. Therefore, in the analysis of
the temperature dependence of the conductivity reported by
*Bubnova et al. [*3] we will rely on the Monte Carlo results
*only. It is noteworthy that Li et al. [*37] discussed recently
the limitations of the semianalytical approaches based on the
transport energy concept.

**B. Comparison with experimental data**

In this section we will use the semianalytical approach to fit systematically the experimental data reported by Bubnova

*et al. [*3] and to extract the physical parameters of the
*system such as an extension of the localized state α, and the*
*broadening of the DOS σ*DOS.

FIG. 2. Comparison of the semianalytical calculations of (a) the
Seebeck coefficient and (b) the conductivity with the experimental
results of Ref. [3]. Solid lines are semianalytical calculations; filled
symbols correspond to the original experimental data as a function
*of the relative oxidation level nox*; open symbols in the grey-shaded

region corresponds to experimental data with the rescaled density
*of free carriers n= bnox* as discussed in the text. The extracted

*concentration dependence of the parameter b is shown in the*
*inset. σ*DOS*= 4kT , T = 300 K (Gaussian DOS is used); α = 1.5a,*

*ν*0= 1012s−1.

Let us first note that the conductivity and the Seebeck
coefficient in Ref. [3] are measured as a function of the
*oxidation level nox*. It has been argued by Kim and Pipe [23]
that in similar conducting polymers a fraction of free carriers
contributing to the transport can be orders of magnitude
*smaller than the oxidation level if nox*is low. Our results
sup-port this conclusion for a PEDOT electrochemical transistor
studied in Ref. [3]. Indeed, Fig.2(a)shows a comparison of the
experimental data and the calculated Seebeck coefficient for
the Gaussian DOS [Eq. (3*)] using parameters α, σ*DOS*, and ν*0
providing the best fit between the theory and experiment in the
*concentration range n/N*0* 0.2. (A determination of α, σ*DOS,
*and ν*0 will be discussed in more detail later in this section.)
*While for a high relative concentration n/N*0* 0.2 one can*
achieve a perfect fit between the theory and experiment, no
*such fit is possible for n/N*0* 0.2. Note that we checked that*
this conclusion holds for other functional dependencies of the
DOS, such as an exponential, constant, and power-law DOS.
The agreement between the theory and experiment can be
*restored if we assume that only a fraction of carriers b*= *n*

*nox*
participates in the transport. Comparing the theoretical curve
*with the experimentally measured S, we extract the density*
*dependence of the parameter b as shown in the inset to*
Fig. 2(a). The experimental data, rescaled to the effective
*density n= bnox,*is plotted in Fig.2using the best fit obtained
*from the dependence b= b(nox).*

The difference between the number of free carriers and the oxidation level was attributed by Kim and Pipe [23] to the fact that not all ionized dopants contribute mobile carriers. While this might be true for the material systems discussed in their work, this explanation can hardly be applied

FIG. 3. Visualization of transport paths in 50×50×50 lattice calculated by the Monte Carlo technique for small and large carrier
*concentrations, (a) n/N*0= 10−7*, (b) n/N*0*= 0.35 Temperature T = 300 K; Gaussian DOS with α = a; σ*DOS*= 4kT , T = 300. The magnitude*

of current is coded by both the thickness and filling as indicated in the inset.
to the electrochemical transistor studied in Ref. [3]. Indeed, in
the electrochemical transistor the oxidation level is changed
(decreased) by the application of the positive gate voltage
to the electrolyte covering PEDOT (see Refs. [3,4,20] for
the description of the electrochemical transistor operation).
*A change of the gate voltage Vg*does not affect the ionization
of dopants (deprotonated sulfonyl groups SO−_{3}). Instead, the
positively charged ions (Na+) are forced from the electrolyte
into PEDOT thus reducing the concentration of free carriers
(polarons and/or bipolarons) there. Because of the capacitative
nature of the gate action, the concentration of positive
ions is proportional to the gate voltage and, therefore, the
*concentration of free carriers (i.e., the oxidation level nox*)
*is expected to decrease linearly with the increase of Vg*. The
*dependence n= bnox*[inset to Fig.2(a)] shows, however, that
for low carrier densities a number of free carriers participating
*in the transport, n, deviates strongly from nox*. We speculate
that this behavior can be related to the morphology of the
material system and the percolative character of the hopping
transport in the disordered lattice. To illustrate this we visualize
in Fig.3charge carriers transport paths in 50×50×50 lattice

calculated by the Monte Carlo technique for large and small carrier concentrations. For the case of the large concentration the transport paths essentially form a homogeneous three-dimensional network. As the concentration is reduced, the three-dimensional network gradually transforms into quasi-one-dimensional percolation chains. With the increase of the concentration of positive ions in the polymer one can expect that an increasing fraction of the charge carriers will be blocked by positive ions in finite chain segments.

Also, the system at hand contains a significant number of carriers executing so-called soft jumps where the carriers are trapped for a very long time within clusters of several sites, which are energetically and/or spatially removed from the remaining sites. These carriers would apparently contribute to the overall oxidation level, but they would not contribute to the transport. An additional reason for the difference between

*nand nox*can be related to the Andersson localization, which
can take place for high disorder concentration (i.e., high
concentration of Na+ ions) and which can therefore lead to
blocking of the transport at the low charge density. More
studies are needed in order to resolve this question; work is in
progress in order to model the effect of the morphology and the
*disorder by means of the Monte Carlo and ab initio calculations*
in the presence of disorder. It would be also interesting to see
how the density dependence of the mobility is affected by the
fact that the number of carriers contributing to the transport
deviates from the measured oxidation level. In particular,
more accurate measurements of the actual concentration in
experimental samples would help to clarify this issue.

Let us now discuss a determination of the parameters of the
*theory α, σ*DOS*, and ν*0as well as the shape of the DOS from
the comparison with the experimental data. Because of the
*difference between n and nox*discussed above, only the interval
*of the relative carrier concentration n/N*0* 0.2 is used to fit*
*the experimental data; in the remaining interval n/N*0* 0.2*
we rescale the electron density for the experimental data
*as described above. We extract α and σ*DOS by fitting the
*semianalytical results for the Seebeck coefficient S, and*
*then determine ν*0 using the semianalytical prediction for the

*FIG. 4. (Color online) (a)–(b) The Seebeck coefficient S and (c)–(d) the conductivity σ as a function of the relative concentration n/N*0

*calculated by the semianalytical model for the Gaussian and exponential DOS. Open squares show experimental data for S and σ from*
Ref. [3*]; νsa*

0 = 1012s−1(a) and 5×1011s−1*(b). The charge carrier density in the experimental data is rescaled as n= bnox*; the inset shows

*the density dependence of the parameter b obtained as outlined in the text (see discussion of Fig.*2). (The gray background corresponds to the
density interval for which the experimental data is rescaled). Gray squares and corresponding gray lines show the Monte Carlo calculations
*with the parameters α and σ*DOS*corresponding to the best fit for the semianalytical calculations; the Gaussian DOS: α= 1.5a, σ*DOS*= 4kT ,*

*νMC*

0 *= 1.1×10*13s−1*; the exponential DOS: α= 2a, σ*DOS*= 3kT , ν*0*MC= 3.6×10*12s−1*; T* = 300 K. Arrows in (c) and (d) mark concentrations

used for the calculation of the temperature dependence of the conductivity shown in Fig.5.
*conductivity σ . It should be stressed that this fitting provides*

*unambiguous determination of α and σ*DOS. This is because the
*variation of σ*DOSchanges the slope of the Seebeck coefficient,
*whereas variation of α shifts the curve along the x axis leaving*
the slope practically unaffected, see Figs. 4(a), 4(c). (Note
*that S is independent of ν*0 *which means that ν*0 can be
*unambiguously extracted from the conductivity σ .)*

Figures4(a),4(b)and4(c),4(d)show a comparison of the experimental and theoretical results for the Gaussian and the exponential DOS. Both of them reproduce the experimental data rather well giving similar parameters of the theory,

*α= 1.5a, σ*DOS*= 0.1 eV = 4kT (T = 300 K), ν*0= 1012s−1
*(Gaussian DOS), and α= 2a, σ*DOS*= 0.075 eV = 3kT , ν*0=
5×1011_{s}−1 _{(exponential DOS). The values of σ}

DOS agrees
well with the generally assumed disorder strength in organic
semiconductors [25,38*]. The obtained localization length α is*
an order of magnitude greater than the one typically used in
the hopping models for disordered organic materials [26,38].
Large localization lengths obtained from our fitting are in
agreement with those reported by Kim and Pipe [23] for
pentacene field-effect transistor [39], pentacene films [40],
and PEDOT:Tos [4*], where they also found α≈ 1.5–2a.*
*In our calculations we used the lattice constant a*= 1 nm.
*Hence, the localization length α= 1.5–2a corresponds to the*
localized state in the hopping model [Eq. (1)] extended over
2–3 PEDOT monomers (one monomer spans over*≈0.8 nm).*
This is similar to a spatial extend of polarons/bipolarons
in polymer chains predicted by semiempirical [41,42] and

*ab initio calculations [*43,44]. This finding is therefore
con-sistent with a hopping model where the localized states
cor-respond to the polaron/bipolaron quasiparticles extended over
several monomer units. It is noteworthy that the obtained

pa-rameters of the system correspond to large localization lengths,

*α∼ a, when the agreement between the Monte Carlo and*

the semianalytical approach is the best (see Sec.III A). The corresponding results of the Monte Carlo simulations with the parameters obtained from the semianalytical fitting are shown for the comparison in Fig.4.

Note that the experimental results [3] show not only a
smooth monotonic decrease (increase) of the Seebeck
coef-ficient (conductivity) as a function of the carrier density, but
also some fine structure and bumps in the above dependencies.
This fine structure apparently can not be described by a single
trial DOS (such as the Gaussian or exponential). We have tried
a superposition of several DOS functions and were able to
achieve better agreement with the experimental results (not
shown here). However, a detailed search for the hopping
parameters and the DOS distribution to obtain a quantitative
agreement is problematic. In addition, more experimental
work is needed to ensure that the observed bumps in the
*dependencies of S and σ are systematic features of PEDOT*
films. Note that a complicated kinklike DOS dependence was
directly measured for the organic tetrathiafulvalene field-effect
transistor in Ref. [45]. For conducting polymers OCC-PPV and
P3HT in the regime of the low electron density the shape of
*the DOS was estimated by Oelerich et al. [*46] to be Gaussian.
Paulsen and Frisbie [47] have shown that the DOS of the
P3HT in the high-density regime was more complex in shape
and can be approximated with no fewer than four Gaussians
with numerous heads and shoulders.

Finally, let us discuss the observed temperature dependence of the conductivity. Figure5shows a comparison of the Monte Carlo calculations and the experimental results of Bubnova

200 250 300 350 ) m c/ S( 300 320 340 360 380 400 200 250 300 350 T (K) ) m c/ S( exponential DOS (a) (b) Gaussian DOS

FIG. 5. Monte Carlo calculations of the temperature dependence
of the conductivity for the (a) Gaussian and (b) exponential DOS.
The experimental data of Ref. [3] is shown by open squares. The
*parameters α, σ*DOS*, and ν*0 are given in caption to Fig. 4. The

calculations are performed for the relative concentration _{N}n

0 *≈ 0.3*

marked by arrows in Fig.4, which corresponds to the experimental concentration of Ref. [3]. Averaging is done over 96 samples.

*σ∝ exp (−Ea/kT) with the activation energy Ea=30.3 meV.*
This behavior is rather well reproduced by the Monte Carlo
*calculations giving Ea* *= 27.5.6 meV for the Gaussian DOS*
and 23 meV for the exponential one.

Note that for lower temperatures the model of hopping transport used in this study represents the basis of the classical variable-range hopping theory developed by Mott and leading to the well-known predictions for the conductivity,

*σ* *∝ exp (−[T*_{0}*/T*]*1/(d*+1)*), where d is the dimensionality of*
the system [31]. At temperatures higher than a certain critical
temperature [30] the Mott dependence is replaced by the
activation behavior that is reproduced in our study. Shklovskii
and Efros [31] have demonstrated that the electron-electron
interaction can open the Coulomb gap in the DOS, which
leads to the temperature dependence of the conductivity
*described by σ* *∝ exp (−[TC/T*]*1/2*). Note that the
Shklovski-Efros dependence can be seen in the conductance at very low
temperatures only because the Coulomb gap is smeared by the
temperature already at few Kelvin. Recently, a crossover from
the Shklovski-Efros dependence to the Mott dependence has
*been reported for poly(3-hexylthiophene) by Wang et at. [*48].

**C. Effect of dimensionality**

We modeled PEDOT structure as a three-dimensional (3D) lattice. It is known that ideal PEDOT crystals form an ordered stacked structure [49,50] with different distances between the planes in different directions. It is also plausible that realistic experimental structures [3,15,19] can be composed of regions with short-range order with dominating transport in two dimensions (within the planes) or in one dimension (along the chains). It is therefore of interest to investigate how the dimensionality of the motion affects the observed properties of the system at hand. In this section we report

0 100 200 300 400 500 600 1E-3 0.01 0.1 1 10 100 1E-3 0.01 0.1 1 1 2 3 4 ) K/ V m( | S| ) m c/ S( r

Relative carrier concentration n/N_{0}

3D 2D 1D (a) (b) (c) n

FIG. 6. (Color online) The concentration dependence of (a) the
*Seebeck coefficient S, (b) the conductivity σ , (c) the average hopping*
distance*r for the cases of 3D, 2D, and 1D motion calculated using*
*the Monte Carlo technique. Temperature T* = 300 K; Gaussian DOS
*with α= 1.5a; σ*DOS*= 4kT , and ν*0*= 2.5×10*12s−1. 50×50×50

lattice was used for 3D calculations; 50×50 lattice was used for 2D
calculations; and 50-sites long chain was used for 1D calculations.
*Dashed line in (b) shows a functional dependence σ∝ n.*

the results of the Monte Carlo calculations for the Seebeck coefficient and conductivity for the cases of two-dimensional (2D) and one-dimensional (1D) motion. The theoretical results allow one to draw a general conclusion on the effect of the reduced dimensionality and might serve as the basis for a further analysis of more complicated morphologies.

The Seebeck coefficient and the conductivity for the cases
of 3D, 2D, and 1D motion are shown in Fig.6as a function
of the carrier concentration. For all cases the conductivity
*exhibit very similar functional dependencies, close to σ* *∝ n*
with deviations from this behavior being most pronounced
for the 1D case. As expected, for a given concentration the
absolute value of the conductivity is largest for the 3D case
and decreases as the dimensionality is reduced. The Seebeck
coefficients for all dimensionalities show the same functional
*dependence, and the absolute values of S are rather close for*
3D, 2D, and 1D cases. The average hopping distance *r*
is shown in Fig.6. We find that *r ≈ 3a being practically*
*independent on both n and dimensionality. For the system at*
hand this hopping distance corresponds to jumps over 3–4
PEDOT unit cells.

We mentioned above that in the variable range hopping regime (corresponding to the case of the hopping transport at low temperatures) the temperature dependence of the

conductivity is different for the cases of 3D, 2D, and 1D
transport [31]. This allows one to draw a conclusion about the
dimensionality of the system under study from the temperature
measurements. Our findings demonstrate that a concentration
dependence of the Seebeck coefficient and conductivity can not
be used to obtain information about the dimensionality of the
transport. On the other hand, the insensitivity of the functional
*dependence S= S(n) and σ = σ (n) on the dimensionality*
justifies the use of 3D lattice for the Monte Carlo calculations.

**IV. CONCLUSIONS**

In this work we present a theoretical analysis of the
thermoelectric properties of the electrochemical transistor
*reported by Bubnova et al. [*3]. In order to calculate the
conductivity and the Seebeck coefficient for the system at hand
we adopt a standard model of the phonon-assisted hopping
transport and perform extensive Monte Carlo calculations
complemented by a semianalytical treatment employing the
concept of the transport energy.

Our main findings can be summarized as follows:

(i) We perform the Monte Carlo calculation of the Seebeck
coefficient for the hopping transport in a disordered organic
material. We find that the Monte Carlo and the
semiana-lytical approaches show a good qualitative agreement for
the concentration dependence of the conductivity and the
Seebeck coefficient. We find that the above agreement depends
*primarily on the localization length α in the hopping model:*
*the larger α, the better the agreement. In particular, we find*
that when the localization length is of the order of the lattice
constant, the agreement between the Monte Carlo and the
semianalytical approaches becomes almost quantitative. At
the same time, we find that the semianalytical approach is not
in a position to describe the temperature dependence of the
conductivity.

(ii) In contrast to the exact Monte Carlo calculations, the semianalytical approach does not demand extensive com-putational resources. This allows us to use this approach to perform a systematic analysis of the experimental data and extract parameters of the system at hand. Using this approach to extract the experiment data from the concentration dependence of the the Seebeck coefficient and conductivity we find that both Gaussian and exponential DOS reproduce the experimental data rather well giving similar parameters of the theory. In particular, we find that the localization length

*α≈ 1.5 nm, disorder strength σ*DOS*≈ 0.1 eV = 4kT (at T =*
*300 K) and attempt-to-escape frequency ν*0≈ 1012s−1. The
average hopping distance obtained from the Monte Carlo
calculations is *r ≈ 3 nm. The fitting of the experimental*
data suggests therefore a hopping model where localized states
correspond to the polaron/bipolaron quasiparticles extended
over 2–3 PEDOT monomer units with typical jumps over a
distance of 3–4 monomer units.

(iii) We find that for a low carrier concentration a number of free carriers contributing to the transport deviates strongly from the measured oxidation level. While this finding is in agreement with the previous result reported for similar con-ducting polymers, for the electrochemical transistor studied in Ref. [3] we propose here an alternative interpretation.

(iv) Using the Monte Carlo calculation we reproduce the activation behavior of the conductivity with the calculated activation energy close to the experimentally observed one.

(v) We study the effect of the dimensionality on charge
transport calculating the Seebeck coefficient and the
conduc-tivity for the cases of 3D, 2D, and 1D motion. For all cases
the conductivity exhibits very similar functional dependence,
*close to σ* *∝ n; a deviation from this behavior is most*
pronounced for the 1D case. The Seebeck coefficients for all
dimensionalities also show the same functional dependence,
*and the absolute values of S are rather close for 3D, 2D, and*
1D cases.

*(vi) The expressions for the Seebeck coefficient S available*
in the literature [29,30,32] are usually derived within the
relaxation time approximation in the assumption of the band
transport. In this study we present a general derivation of
the Seebeck coefficient without a relation to any particular
mechanism of transport.

**ACKNOWLEDGMENTS**

We are grateful to M. Kemerink for helpful discussions. The research was supported by the Energimyndigheten, the European Research Council (ERC-starting-grant 307596), and the Knut and Alice Wallenberg Foundation (The Tail of the Sun).

**APPENDIX A: DERIVATION OF THE SEEBECK**
**COEFFICIENT S**

*Expressions for the Seebeck coefficient S available in the*
literature [29,30,32] are usually derived within the relaxation
time approximation in the assumption of the band transport.
*It is therefore not a priori evident how and whether these*
expressions can be used for the description of the hopping
motion. In this appendix we present a general derivation of
the Seebeck coefficient without a relation to any particular
mechanism of transport including the hopping one.

We start by expressing the Seebeck coefficient via the
*electrical current, J , and the energy current, Jε*[29,30,32],

*S*= *Jε− μJ*

*−|e|T J* *.* (A1)

*Express J and Jε* *in a standard way as J* *≡ J = Tr{ρ ˆJ},*

*Jε≡ Jε = Tr{ρ ˆJε}, where ρ is the statistical operator for the*
Hamiltonian ˆ*H, ρ* =* _{Z}*1

*e*−

*kTH*ˆ

*, Z*=

*ne*−

*En*

*kT*, ( ˆ*H|n = E _{n}|n),*
and the quantum-mechanical particle and energy currents are

ˆ

*J* *= ˆJk*= * _{V}*1

*vk*, ˆ

*Jε= εkJ*ˆ

*k*=

*1*

_{V}*εkvk*[29,32

*] (V is the volume,*

*v*is the velocity).

Consider a perturbed system, *ρ= ρ*0*+ δρ, where*

*ρ*_{0} corresponds to the equilibrium situation when no
current flows, Tr*{ρ*0*J*ˆ*} = 0. (Note that ρ*0*|ψE = fF D|ψE*,
*where fF D* *stands for the Fermi-Dirac distribution fF D* =

1

1*+exp [(E−FF)/kT ]*.) Then Tr{ρ ˆJ} =

*kkk|δρ|kk| ˆJk|k =*
1

*V|e|T*

*dEdEg(E)g(E*)E*|δρ|EE|v|E*, and Eq. (A1)
reads,

*S*= −

*dEdEg(E)g(E*)ψ*E|δρ|ψEψE|(E − μ)v|ψE*
*|e|T**dEdEg(E)g(E*)ψ*E|δρ|ψEψE|v|ψE*

*,*

*where g(E) is the density of states (DOS), and ψE* is the
eigenfunction of the Hamiltonian ˆ*Hat the energy E.*

Let us now specify the perturbation of the sys-tem. Assuming a harmonic variation of the form

*δρ(t)= δρe−iωt+αt, δ ˆH(t)= δ ˆH e−iωt+αt(and letting α*→ 0)
one can show that [32]

*ψE|δρ|ψE* =

*fF D(E*)*− fF D(E)*

*E− E − ω − iαψE|δ ˆH|ψE. (A3)*

*The system responses to the change of the electric field F ,*
*which is, in turn, related to the vector potential A= A*0*+ δA*
*as F* = −* _{∂t}∂(δA), such that δ ˆH* = −

*|e|F v*[32]. Using the

_{iω}*representation of the δ function Re(limα*→0

*1 )=*

_{E}_{−E−ω−iα}*iπ δ(E− E − ω) and considering limit ω → 0 when*

*fF D(E+ω)−fF D(E)*

*ω* =

*∂fF D*

*∂E* *, we obtain from Eqs. (*A2), (A3)

*S(T )*= − 1
*|e|T*
*dE(E− EF)σ (T ,E)*
−*∂fF D*
*∂E*
*σ(T )* *,* (A4)
*σ(T )*=
*dEσ(T ,E)*
−*∂fF D*
*∂E*
*,* (A5)

*σ(T ,E)= 2e*2*πV |g(E)|*2*ψE|v|ψE*2*,* (A6)
where factor 2 in Eq. (A6) accounts for spin. Note that
*expressions for S(T ) and σ (T ), Eqs. (*A4), (A5), are
for-mally identical to corresponding equations in Ref. [29]
*(ch. 13) where, however, σ (T ,E) is expressed via Boltzmann’s*
relaxation time (which is appropriate for the case of band
*transport). We point out that our expression for σ (T ,E) [given*
by Eq. (A6)] is not limited to any particular mechanism of
transport.

Let us focus on the expression for the conductivity, Eq. (A6), and rewrite it in alternative forms corresponding to the Kubo-Greenwood formula and the Einstein relation. Substituting Eq. (A6) into Eqs. (A4), (A5) and changing an integration over energy into summation over all available states

*k* we obtain for the nominator and denominator of Eq. (A4)
(upper and lower rows in the square brackets correspondingly),

*2e*2*πV*
*dE*
*(E− EF*)
1
*|g(E)|*2_{ψ}*E|v|ψE*2
−*∂f*0
*∂E*
(A7)
= *2e*2*π*
*V*
*k,k*
*vkkvkk*
*(Ek− EF*)
1
*δ(Ek− Ek*)
−*∂f*0
*∂E*
(A8)
= *2e*2*π*
*V*
∞
−∞
*dE*
*(E− EF*)
1
*k,k*
*vkkvkk*
*× δ(E − Ek)δ(E− Ek*)
−*∂f*0
*∂E*
(A9)
= *2e*2*π*
*V*
∞
−∞
*dE*
*(E− EF*)
1
*Tr[vδ(E*− ˆ*H)vδ(E*− ˆ*H*)]
×
−*∂f*0
*∂E*
*,* (A10)

where in Eq. (A9*) we utilized the identity δ(Ek− Ek*)=
_{∞}

−∞*dE δ(E− Ek)δ(E− Ek*), and in Eq. (A10) we used a
definition of the trace. It follows from Eq. (A10) that the
*definition of σ (T ,E) in Eqs. (*A4)–(A6) can be reduced to
the standard Kubo-Greenwood formula [32],

*σ(T ,E)*=*2e*

2_{π}_{}

*V* *Tr[vδ(E*− ˆ*H)vδ(E*− ˆ*H)].* (A11)

It is worth mentioning that the Kubo-Greenwood formula transforms to a familiar expression for the conductivity corresponding to the Einstein relation [35,36],

*σ(T ,E)= e*2*g(E)D(E),* (A12)
where the diffusion coefficient is given by the mean quadratic
spreading

*D(E)*= lim
*t*_{→∞}

*( ˆX(t) − ˆX(0))*2_{}

*t* *,* (A13)

with ˆ*X(t) being the position operator in the Heisenberg*
representation.

**APPENDIX B: SEEBECK COEFFICIENT IN THE**
**SEMIANALYTICAL APPROACH WITHIN THE**

**TRANSPORT ENERGY CONCEPT**

In this appendix we briefly outline formulas that we use to
calculate the Seebeck coefficient within the transport energy
*concept based on the results of Schmechel et al. [*22]; note that
a similar approach was also used by Kim and Pipe [23].

Start by introducing the (differential) escape rate
*distribu-tion νesc* *(E*0*,W) for an electron on the energy E*0*+ W (where*

*E*0is the initial state),

*ν _{esc}*

*(E*0

*,W*)=

*ν*0

*kT*exp

*− 2αR(E*0

*+ W) −*

*W*

*kT*

*,*(B1)

where *R*¯*(E) is the mean distance that has to be *
*over-come by an electron of energy E by tunneling, ¯R(E)*=
(_{3B}4π_{−∞}*E* *g(ε)[1− fF D(ε)]dε)*

*−1/3*

*. In the last expression B*
is a parameter that accounts for a percolative character of
*hopping transport in a disordered system; it was chosen B*= 1
in Ref. [22*] and B= 2.7 in Ref. [*23]. Introduce the differential
*conductivity σ(E)= en(E)μ(E) and the differential particle*
*density n(E)= g(E)fF D(E) such that*

*σ* =
_{+∞}
−∞
*σ(E) dE,* (B2)
*n*=
_{+∞}
−∞
*n(E) dE.* (B3)
[As follows from Eq. (A5), the relation between the
*dif-ferential conductivity and the conductivity σ (E,T ) used in*
the Monte Carlo calculations [Eqs. (A6), (A8), (A12)] is

*σ= σ (T ,E)(−∂fF D*

*∂E* *).] The mobility μ(E) is given by the*
generalized Einstein relation

*μ(E)*= *|e|*

*where η is a fitting constant, and the diffusion coefficient is*
given by

*D(E)= λ*2*(E)νesc(E),* (B5)

*where λ(E)= R[Eesc(E)] is the carrier mean jump distance*
*at energy E, νesc(E) is the total escape rate of an electron from*
*the state with the energy E*

*νesc(E)*=
_{+∞}

0

*ν _{esc}*

*(E,ε) dε,*(B6)

*Eesc(E) is the mean energy at which a carrier is released from*
*an initial state at the energy E,*

*Eesc(E)= E +*
_{+∞}
0 *ενesc* *(E,ε) d*
_{+∞}
0 *νesc* *(E,ε) d*
*.* (B7)

It is noteworthy that the definition of the diffusion coefficient,
Eq. (B5), is consistent with the definition based on Eq. (A13)
*where the square of the mean jump length during time τ* *= ν*−1_{esc}*corresponds to the mean quadratic spreading during time t.*

Finally, the Seebeck coefficient is given,

*S(T )*= − 1
*|e|T*
*dE(E− EF)σ(E)*
*σ(T )* =
*EF− E*trans
*|e|T* *,* (B8)
*where the transport energy E*trans is the averaged energy
weighted by the conductivity distribution,

*E*trans=

*εσ() dε*

*σ(T )* *.* (B9)

**APPENDIX C: KINETIC MONTE-CARLO METHOD**

This section describes the main steps in the simulation
of the hopping transport based on the kinetic Monte Carlo
method [25,26,51]. The method includes a definition of a
lattice, assigning energy levels to every site according to the
chosen DOS, and then running the simulation by monitoring a
random walk of charge carriers between the sites. In our
calcu-lations we do not account for electron-electron interaction
ex-cept allowing no more than one electron to occupy a single site.
*The organic semiconductor is modeled by a 3D Nx×Ny*×

*Nzlattice with a lattice constant a where the periodic boundary*
conditions are chosen in all directions. For a given lattice
configuration a random walk of typically 10 charge carriers
is simulated. This is known to be a reasonable compromise
between computer time and computational statistics [25]. It is
worth noting that in our model the Fermi energy is explicitly
defined, which means that the charge carrier concentration is
given not by the above number of carriers but by the number
of sites occupied according to the Fermi-Dirac statistics for
*a given EF*. Several lattice configurations (typically 16) with
different disorder realizations are used to obtain statistically
*averaged quantities of σ and S.*

In order to generate a current we apply a small potential
*difference V to the boundaries of the sample in the x direction*
(|e|V = k*BT /*10). The energy on the site with the coordinate

*xi* *transforms into Ei* *→ Ei− |e| _{L}V_{x}xi, where Lx* is the size

*of the computational domain in the x direction. Because we*assume a local equilibrium, the Fermi energy drops linearly

*between E*left

*F*

*and E*right

*F*

*= E*left

*F*

*− |e|*

*V*

*Lx*. Apparently, with

*this transformation, the difference Ei− EF*remains locally unchanged under an application of the external voltage.

The kinetic Monte Carlo simulation proceeds as follows.
*(i) Initialization of site energies Ei. For every site i, a*
random value of the energy is drawn from a Gaussian or
exponential DOS, Eqs. (3), (4). To facilitate generation of the
random energies the Metropolis-Hastings algorithm is used.

*(ii) Initial placement of charges. N*charges charges whose
dynamics will be explicitly traced are randomly placed on the
lattice according to the Fermi-Dirac occupation probabilities.
(iii) Choice of hopping events. First, using Eq. (1), we
*calculate all the hopping rates νijfrom the sites i where charges*
have been placed on the previous step. To prevent hopping into
already occupied sites, we set corresponding hopping rates
equal to 0. Because the hopping rate decreases exponentially
with the distance, it is possible to introduce a cut-off distance
*and set νij* = 0 for the jumps longer than this distance. This
reduces substantially the computational time and resources.
We have checked that for the parameters and regimes studied
in the present work, practically no jumps occur between sites
*separated by the distance 6a and we thus use this value as the*
cut-off distance.

*We renormalize the hopping rates ij* introducing
*corre-sponding probabilities, pij*,
*pij* =
*ij*
*ijij*
*.* (C1)

In the above sum we include only jumps from the occupied
*to unoccupied sites, i.e., we set ij* *= 0 if site j is occupied*
*or site i is empty. Then, for each charge, we randomly choose*
a hopping event with a probability equal to Eq. (C1) using a
following algorithm. First, we enumerate all hopping events
*introducing for every pair ij an index k (i.e., ij* *→ k, and*

*pij* *= pk), where k∈ {1, . . . ,k*max*}, with k*max being the total
*number of all possible hopping events. Then a partial sum Sk*
*is defined for every index k*

*Sk* =
*k*
*k*=1

*pk.* (C2)

*Apparently, for every k the length of the interval [Sk*_{−1}*,Sk*] is
*equal to the probability pkfor the kth jump, and the total length*
*of all intervals is equal to 1, i.e., Sk*max= 1. Then we draw a

*random real number r from the interval [0,1] and find the index*

*ksuch that Sk*−1* r Sk*, which gives us the hopping event
that will occur. Having chosen the hoping event we move a
*charge between the corresponding sites i and j .*

(iv) Calculation of the waiting time. After every hopping
*event, we add to the total simulation time t the waiting time τ*
that has passed until the event took place. This time is obtained
by drawing a random number from the exponential waiting
*time distribution P (τ )= νi*exp[−ν*iτ] with νi*=

*jνij*being
*the total hopping rate of hopping from site i. It is therefore*
given by

*τ* = −1
*νi*

*ln r,* (C3)

*where a random number r is drawn from the interval [0,1].*
(v) Calculation of the current density. Every time that a
predefined number of jumps has occurred, we calculate the

*current density, J (t), via the following expression*

*J(t)*= *e(N*

+* _{− N}*−

_{)}

*t NyNza*2

*,* (C4)

*where N*+ *and N*− are the total number of jumps along and
*against the electric field for a cross section slice in the yz plane.*
*We keep track of the time evolution of the current density J (t)*
*and stop the calculation when a converged current J has been*
obtained. This usually takes several million hopping events.
Note that following the standard practice we exclude from the
*calculations Nin* *initial hopping events (typically Nin*∼ 104)
[26] because they can give an extreme contribution to the
*current and thus lead to incorrect J .*

(vi) Calculation of the conductivity and the Seebeck
*coefficient. The conductivity σ is obtained from σ* = * _{F}J*,

*where the electric field F*= _{L}V

*x*. The Seebeck coefficient is
computed according to Eq. (5), which requires a computation
*of the transport energy E*trans. According to Eq. (6) the
transport energy defines the energy of states that conduct
the current most efficiently [22]. In our calculations we
store the energy levels over which carriers jump and determine

*E*trans *from the analysis of the current density J as a*

function of the energy. Note that in the calculation of the current and the transport energy we exclude a contribution of so-called soft jumps where charges are trapped for a long time in the pairs of spatially and energetically close sites [52].

Finally, we have confirmed a validity of the implemented Monte Carlo algorithm by comparing the calculated results with the available data in the literature [25].

[1] O. Bubnova and X. Crispin,**Energy Environ. Sci. 5**,9345(2012).
[2] Y. Xuan, X. Liu, S. Desbief, P. Leclere, M. Fahlman, R.
Lazzaroni, M. Berggren, J. Cornil, D. Emin, and X. Crispin,
**Phys. Rev. B 82**,115454(2010).

[3] O. Bubnova, M. Berggren, and X. Crispin,J. Am. Chem. Soc.

**134**,16456(2012).

[4] O. Bubnova, Z. U. Khan, A. Malti, S. Braun, M. Fahlman, M.
Berggren, and X. Crispin,**Nat. Mater. 10**,429(2011).

[5] T. Park, C. Park, B. Kim, H. Shin, and E. Kim,Energy Environ.
**Sci. 6**,788(2013).

[6] T.-C. Tsai, H.-C. Chang, C.-H. Chen, Y.-C. Huang, and W.-T.
Whang,**Org. Electronics 15**,641(2014).

[7] M. Culebras, C. M. Gmez, and A. Cantarero,**Materials 7**,6701
(2014).

[8] L. Groenendaal, F. Jonas, D. Freitag, H. Pielartzik, and J. R.
Reynolds,**Adv. Mater. 12**,481(2000).

[9] M. V. Fabretto, D. R. Evans, M. Mueller, K. Zuber, P.
Hojati-Talemi, R. D. Short, G. G. Wallace, and P. J. Murphy,
**Chem. Mater. 24**,3998(2012).

[10] O. Bubnova, Z. U. Khan, H. Wang, S. Braun, D. R. Evans,
M. Fabretto, P. Hojati-Talemi, D. Dagnelund, J.-B. Arlin, Y. H.
Geerts, S. Desbief, D. W. Breiby, J. W. Andreasen, R. Lazzaroni,
W. Chen, I. Zozoulenko, M. Fahlman, P. J. Murphy, M. Berggren,
and X. Crispin,**Nat. Mater. 13**,190(2014).

[11] S. Stafsr¨om,**Chem. Soc. Rev. 39**,2484(2010).

[12] J. Hwang, D. B. Tanner, I. Schwendeman, and J. R. Reynolds,
**Phys. Rev. B 67**,115205(2003).

[13] S. K. M. J¨onsson, J. Birgerson, X. Crispin, G. Greczynskib,
W. Osikowicz, A. W. Denier van der Gon, W. R. Salaneck, M.
Fahlman,**Synth. Met. 139**,1(2003).

[14] X. Crispin, F. L. E. Jakobsson, A. Crispin, P. C. M. Grim,
P. Andersson, A. Volodin, C. van Haesendonck, M. Van der
Auweraer, W. R. Salaneck, and M. Berggren,**Chem. Mater. 18**,
4354(2006).

[15] A. M. Nardes, M. Kemerink, R. A. J. Janssen, J. A. M.
Bastiaansen, N. M. M. Kiggen, B. M. W. Langeveld, A. J. J.
M. van Breemen, and M. M. de Kok,**Adv. Mater. 19**, 1196
(2007),

[16] A. M. Nardes, R. A. J. Janssen, and M. Kemerink,Adv. Funct.
**Mater. 18**,865(2008).

[17] A. M. Nardes, M. Kemerink, and R. A. J. Janssen,Phys. Rev. B

**76**,085208(2007).

[18] A. J. Kronemeijer, E. H. Huisman, I. Katsouras, P. A. van Hal,
T. C. T. Geuns, P. W. M. Blom, S. J. van der Molen, and D. M.
de Leeuw,**Phys. Rev. Lett. 105**,156604(2010).

[19] N. Kim, B. H. Lee, D. Choi, G. Kim, H. Kim, J.-R. Kim, J.
Lee, Y. H. Kahng, and K. Lee,**Phys. Rev. Lett. 109**,106405
(2012).

[20] D. Nilsson, M. Chen, T. Kugler, T. Remonen, M. Armgarth, and
M. Berggren,**Adv. Mater. 14**,54(2002).

[21] H. Sirringhaus,**Adv. Mater. 17**,2411(2005).
[22] R. Schmechel,**J. Appl. Phys. 93**,4653(2003).

[23] G. Kim and K. P. Pipe,**Phys. Rev. B 86**,085208(2012).
[24] S. D. Baranovskii,**Phys. Status Solidi B 251**,487(2014).
[25] H. B¨assler,**Phys. Status Solidi B 175**,15(1993).

[26] J. J. M. van der Holst, F. W. A. van Oost, R. Coehoorn, and
P. A. Bobbert,**Phys. Rev. B 83**,085206(2011).

[27] J. Cottaar, R. Coehoorn, and P. A. Bobbert,Organic Electronics

**13**,667(2012).

[28] D. Mendels and N. Tessler,**J. Appl. Phys. 117**,105502(2015).
*[29] N. W. Ashcroft and N. D. Mermin, Solid State Physics (Sounders*

College, Fort Worth, 1976).

*[30] D. Emin, in Wiley Encyclopedia of Electrical and Electronics*
*Engineering Online, edited by J. G. Webster (John Wiley &*
Sons, New York, 2002), pp. 1–44.

*[31] B. I. Shklovskii, A. L. Efros, Electronic properties of doped*
*semiconductors (Springer, Heidelberg, 1984).*

*[32] O. Madelung, Inroduction to Solid-State Theory (Springer,*
Heidelberg, 1996).

[33] A. Miller and E. Abrahams,**Phys. Rev. 120**,745(1960).
[34] M. C. J. M. Vissenberg and M. Matters, **Phys. Rev. B 57**,

12964(1998); J. Nelson,* ibid. 67*,155209(2003); N. Sedghi, D.
Donaghy, M. Raja, S. Badriya, S. Higgins, and W. Eccleston,

**J. Non-Cryst. Solids 352**, 1641(2006); M. Estrada, I. Mejia, A. Cerdeira, J. Pallares, L. Marsal, and B. Iniguez,Solid State

**Electron. 52**,787(2008); M. Tachiya and K. Seki,Phys. Rev. B

**82**,085201(2010).

[35] S. Roche and D. Mayou,**Phys. Rev. Lett. 79**,2518(1997).
[36] F. Triozon, S. Roche, A. Rubio, and D. Mayou,**Phys. Rev. B 69**,

[37] L. Li, N. Lu, and M. Liu, **Europhys. Lett. 106**, 17005
(2014).

[38] R. Coehoorn, W. F. Pasveer, P. A. Bobbert, and M. A. J. Michels,
**Phys. Rev. B 72**,155206(2005).

[39] K. P. Pernstich, B. R¨ossner, and B. Batlogg,**Nat. Mater. 7**,321
(2008).

[40] K. Harada, M. Sumino, C. Adachi, S. Tanaka, and K. Miyazaki,
**Appl. Phys. Lett. 96**,253304(2010).

[41] F. C. Lavarda, M. C. dos Santos, D. S. Galvao, and B. Laks,
**Phys. Rev. B 49**,979(1994).

[42] D. Giri and K. Kundu,**Phys. Rev. B 53**,4340(1996).

[43] A. Dkhissi, D. Beljonne, and R. Lazzaroni, F. Louwet, L.
Groenendaal, and J. L. Br´edas,**Int. J. Quantum Chem. 91**,517
(2003).

[44] A. Dkhissi, D. Beljonne, and R. Lazzaroni,**Synth. Met. 159**,
546(2009).

[45] M. Leufgen, O. Rost, C. Gould, G. Schmidt, J. Geurts, L. W.
Molenkamp, N. S. Oxtoby, M. Mas-Torrent, N. Crivillers, J.
Veciana, and C. Rovira,**Organic Electronics 9**,1101(2008).
[46] J. O. Oelerich, D. Huemmer, and S. D. Baranovskii,Phys. Rev.

**Lett. 108**,226403(2012).

[47] B. D. Paulsen and C. D. Frisbie,**J. Phys. Chem. C 116**,3132
(2012).

[48] S. Wang, M. Ha, M. Manno, C. D. Frisbie, and C. Leighton,
**Nat. Commun. 3**,1210(2012).

[49] E.-G. Kim and J.-L. Br´edas,**J. Am. Chem. Soc. 130**, 16880
(2008).

[50] A. Lenz, H. Kariis, A. Pohl, P. Persson, and L. Ojam¨ae,
**Chem. Phys. 384**,44(2011).

[51] M. Jakobsson and S. Stafstr¨om,**J. Chem. Phys. 135**, 134902
(2011).